(especially magnetic recording)
NSF Workshop on Introducing Science Faculty to
Materials Science and Engineering
June 22, 2009
Professor of Physics
The University of Alabama
Outline of talk
• What is magnetism?
• How can materials be magnetic?
• What are some important properties of
• Magnetic recording – an important
application of nanomagnetism
Maxwell’s equation (SI units):
ρ = charge density
J = current density
ε = permittivity
µ = permeability
E = electric field (intrinsic field)
D = displacement vector = εE (derived field)
B = magnetic induction (intrinsic field)
H = magnetic field = (1/µ)B (derived field)
D = εE = ε0E + P, P = Σp/V = χE = polarization
H = B/µ = B/µ0 – M, or B = µ0(H + M),
M = Σm/V = χmH = magnetization
• SI units: B in tesla (T), H in A/m, M in A/m
• Electromagnetic units (emu): a commonly used cgs
system that works best for magnetism (not the same as the
emu system: B = H + 4πM, B in gauss (G), H in oersted
(Oe), M in Oe (= emu/cm3)
Fields and Units
Currents produce magnetic fields
Long, straight wire current loop (m = IA)
F = qv x B dF = Idl x
Magnetic fields exert forces on
Interaction between a magnetic field and a
magnetic dipole moment
A field exerts a
torque on a magnetic
dipole moment that
tends to align the
dipole in the field
τ = m x B
A non-uniform field
exerts a net force on a
magnetic dipole moment.
F = -m(dB/dz)
orbital: ml = -(e/2m)L
spin: ms = -(e/m)S
Atomic origin of magnetism
Permanent atomic moments in thermal equilibrium
(Boltzmann distribution) in an external magnetic field –
M = n, N = no. atoms per unit volume
= average moment of atom
U = -m.B = -mBcosθ = -mzB
(Quantum mechanics gives similar results.)
Negative magnetic susceptibility exhibited by all
M = χH, (χ < 0)
Based on Faraday’s law: Electronic orbits change when
magnetic field is applied to produce an opposing
magnetic flux. Conduction electrons also exhibit
diagmagnetism. χ is approximately independent of
Spontaneous magnetic ordering
e.g., Co, Fe, Ni, NiFe, CoPt
Caused by exchange interactions between atoms
e.g., Fe3O4 (magnetite),
e.g., MnO, NiO, MnF2,
• Magnetic ordering is due to exchange interaction between
atoms. Exchange energy is the difference between the
Coulomb interaction for antiparallel and parallel electrons
Eex = E↑↑ - E↑↓
• Net wavefunction (spin times
spatial) of two electrons must
be antisymmetrical (Pauli
exclusion principle). Thus,
spatial wavefunction for
parallel and antiparallel spin
configurations must have
different symmetry – further
apart when parallel.
Eex = -2JS1⋅S2,
J = exchange integral
Where in the periodic table do we
FeCo has highest known magnetization
Some Important Properties of Ferro- and Ferri-
•Saturation magnetization – Ms (A/m, emu/cc)
•Magnetocrystalline anisotropy (J/m3, erg/cc)
•Coercivity (A/m, T, Oe)
•Shape anisotropy (J/m3, erg/cc)
Soft Magnetic Materials (low Hc)
• Applications: transformer cores, electromagnetic
cores, read heads, …
• Important properties: Ms (usually want high),
anisotropy (usually low), magnetostriction (usually
small), frequency response (high), eddy current loss
(low resistivity), …
• Examples: Iron and steel, NiFe, CoFe, amorphous
alloys, ferrites, …
• Coercivity depends on both intrinsic properties and
Hard Magnetic Materials (high Hc)
• Applications: permanent magnets, magnetic recording
• Examples: BaFe12O19, Fe14Nd2B, Sm2Co17, CoPtCr, …
• Energy product = (BH)max
• Coercivity depends on anisotropy and microstructure
Large particles and films
generally consist of uniformly
magnetized regions (≥ 0.1 µm)
If particles are
sufficiently small, then
they are ‘single domain’.
Critical size depends on
strength of exchange
shape. DC ~ 10–100 nm.
Domain walls can move
under the influence of an
applied magnetic field.
Hard Disk Drive
Magnetic film on
which bits are stored.
Head for writing and
Servo system for
positioning the head
Magnetic domains oriented in the
direction of travel of the head.
Soft underlayer “mirrors” write
head and makes it possible to
write domains much closer
2012: 4.4 nm x 4.4 nm
The incredible shrinking bit!
Predicted Relative Sizes of HDD Storage Bits
(assumes areal densities continue to double
yearly – but this is no longer occuring)
Typical media layer structure
• diamond-like protection from wear and corrosion
• Co-alloy (CoPtCr, CoPtCrB, CoPtCrTa, …)
• Usually CrX. Helps improve epitaxial growth of
magnetic layer, improves grain isolation by Cr
diffusion from intermediate layer
• grain growth and texture (e.g., CrTi, CrTiB, NiAl)
• helps control grain growth and texture (CrX, e.g.,
• glass or NiP coated Al-Mg. Condition of NiP
coating (oxidation, roughness) has some effect on
Magnetic Media Evolution
grain size (nm)
10 nm mean
11 nm mean
12 nm mean
15 nm mean
9.1 nm mean
9 nm mean
Physical grain size below 10 nm
Ideal Media Structure
traditional lithographically patterned,
• For high-density storage, media should have small, isolated,
thermally stable magnetic grains.
• Small grain size ⇒ magnetization decay; large write versus
store fields ⇒ magnetic anisotropy must be increased.
The problem with small magnets -
• Magnets no longer stay magnetized when they approach the
nanometer size (superparamagnetism)
• Hard drive disks now made of cobalt alloy granular films.
Small size limit is about 8 nanometers.
• One proposed solution for extending storage densities –
Chemically synthesized FePt nanoparticles.
Most materials have a preferred
direction of magnetization.
Usually, due to crystalline structure
(cubic, hexagonal, etc.), shape
(grains, films, etc.), or stress.
Anisotropy energy = energy
difference between “easy” and
Self-organized FePt nanoparticles
• First reported by Sun et al.
[Science, 287, 1989 (2000)] – one
of “Chemistry Highlights” of 2000.
• Synthesis – reduction of Pt(acac)2
in a diol and decomposition of Fe
(CO)5 in presence of surfactant
stabilizers at high temperature.
• Self-assembly – slow evaporation
of particle dispersion on substrate. 3.5 nm FePt particle array –
M. Chen and D.E. Nikles
High Anisotropy FePt Nanoparticle Arrays
• As prepared particles are superparamagnetic.
• Anneal at T ~ 550 oC to produce chemically ordered high-
anisotropy L10 fct phase.
• Particles ≥ 3 nm thermally stable for > 10 years.
• Potential storage density > 1 Tb/in2 as conventional medium
using heat assisted recording.
• Potential storage density ~ 50 Tb/in2 if 1 bit/particle
recording can be achieved.
• Sintering of particles at the high annealing temperatures
required for chemical ordering is a major problem.
Library of Congress,
• the entire printed
collection of the U.S.
Library of Congress
50 terabits per square inch on a half dollar size disk
• Over 3.4 million high-resolution photos, or …
• 2,800 audio CDs, or…
• 1,600 hours of television, or …
Synthesis of FePt Nanoparticles
Courtesy of Hao Zeng (IBM)